 
data_a 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'Fe Mn O6 Y2' 
_chemical_formula_weight          384.59

 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mn'  'Mn'   0.3368   0.7283 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Y'  'Y'  -2.7962   3.5667 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            orthorhombic  
_symmetry_space_group_name_H-M    Pnma 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x+1/2, -y, z+1/2' 
 '-x, y+1/2, -z' 
 'x+1/2, -y+1/2, -z+1/2' 
 '-x, -y, -z' 
 'x-1/2, y, -z-1/2' 
 'x, -y-1/2, z' 
 '-x-1/2, y-1/2, z-1/2' 
 
_cell_length_a                    5.6928(8) 
_cell_length_b                    7.4902(10) 
_cell_length_c                    5.2646(7) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  90.00 
_cell_angle_gamma                 90.00 
_cell_volume                      224.48(5) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     50
_cell_measurement_theta_min       3 
_cell_measurement_theta_max       25 
 
_exptl_crystal_description        flake
_exptl_crystal_colour             black 
_exptl_crystal_size_max           0.03 
_exptl_crystal_size_mid           0.03 
_exptl_crystal_size_min           0.03 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     5.690 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              354 
_exptl_absorpt_coefficient_mu     31.454
_exptl_absorpt_correction_type    multi-scan
_exptl_absorpt_correction_T_min   0.4521 
_exptl_absorpt_correction_T_max   0.4521 
_exptl_absorpt_process_details    'SADABS,2008' 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'CCD area detector' 
_diffrn_measurement_method        'phi and omega scans'
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             1028 
_diffrn_reflns_av_R_equivalents   0.0152 
_diffrn_reflns_av_sigmaI/netI     0.0118 
_diffrn_reflns_limit_h_min        -6 
_diffrn_reflns_limit_h_max        5 
_diffrn_reflns_limit_k_min        -8 
_diffrn_reflns_limit_k_max        8 
_diffrn_reflns_limit_l_min        -6 
_diffrn_reflns_limit_l_max        6 
_diffrn_reflns_theta_min          4.73 
_diffrn_reflns_theta_max          24.99 
_reflns_number_total              215 
_reflns_number_gt                 203 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        'Bruker SMART' 
_computing_cell_refinement        'Bruker SMART' 
_computing_data_reduction         'Bruker SAINT' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0123P)²+0.9279P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    -
_refine_ls_hydrogen_treatment     -
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          215 
_refine_ls_number_parameters      28 
_refine_ls_number_restraints      0 
_refine_ls_R_factor_all           0.0151 
_refine_ls_R_factor_gt            0.0138 
_refine_ls_wR_factor_ref          0.0351 
_refine_ls_wR_factor_gt           0.0345 
_refine_ls_goodness_of_fit_ref    1.178 
_refine_ls_restrained_S_all       1.178 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
O2 O 1.1840(4) 0.5554(3) 0.6966(4) 0.0087(5) Uani 1 1 d . . . 
O1 O 1.0379(6) 0.7500 1.1109(7) 0.0087(8) Uani 1 2 d S . . 
Y1 Y 0.57603(8) 0.2500 1.01782(9) 0.00732(18) Uani 1 2 d S . . 
Mn1 Mn 1.0000 0.5000 1.0000 0.0065(2) Uani 0.50 2 d SP . . 
Fe1 Fe 1.0000 0.5000 1.0000 0.0065(2) Uani 0.50 2 d SP . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
O2 Fe1 1.955(2) . ? 
O2 Mn1 1.955(2) . ? 
O2 Fe1 2.117(2) 2_764 ? 
O2 Mn1 2.117(2) 2_764 ? 
O2 Y1 2.281(2) 2_664 ? 
O2 Y1 2.500(2) 5_767 ? 
O2 Y1 2.624(2) 6_657 ? 
O1 Fe1 1.9733(11) . ? 
O1 Mn1 1.9733(11) . ? 
O1 Fe1 1.9733(11) 3_757 ? 
O1 Mn1 1.9733(11) 3_757 ? 
O1 Y1 2.238(3) 2_665 ? 
O1 Y1 2.300(3) 5_767 ? 
Y1 O1 2.238(3) 2_664 ? 
Y1 O2 2.281(2) 8_756 ? 
Y1 O2 2.281(2) 2_665 ? 
Y1 O1 2.300(3) 5_767 ? 
Y1 O2 2.500(2) 5_767 ? 
Y1 O2 2.500(2) 3_747 ? 
Y1 O2 2.624(2) 4_456 ? 
Y1 O2 2.624(2) 6_557 ? 
Y1 Mn1 3.0563(5) . ? 
Y1 Fe1 3.0563(5) . ? 
Y1 Fe1 3.0563(5) 3_747 ? 
Y1 Mn1 3.0563(5) 3_747 ? 
Mn1 O2 1.955(2) 5_767 ? 
Mn1 O1 1.9733(11) 5_767 ? 
Mn1 O2 2.117(2) 6_557 ? 
Mn1 O2 2.117(2) 2_765 ? 
Mn1 Y1 3.0563(5) 5_767 ? 
Mn1 Y1 3.1840(5) 2_664 ? 
Mn1 Y1 3.1840(5) 6_658 ? 
Mn1 Y1 3.3355(5) 6_657 ? 
Mn1 Y1 3.3355(5) 2_665 ? 
Fe1 O2 1.955(2) 5_767 ? 
Fe1 O1 1.9733(11) 5_767 ? 
Fe1 O2 2.117(2) 6_557 ? 
Fe1 O2 2.117(2) 2_765 ? 
Fe1 Y1 3.0563(5) 5_767 ? 
Fe1 Y1 3.1840(5) 2_664 ? 
Fe1 Y1 3.1840(5) 6_658 ? 
Fe1 Y1 3.3355(5) 6_657 ? 
Fe1 Y1 3.3355(5) 2_665 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
Fe1 O2 Mn1 0.0 . . ? 
Fe1 O2 Fe1 144.44(13) . 2_764 ? 
Mn1 O2 Fe1 144.44(13) . 2_764 ? 
Fe1 O2 Mn1 144.44(13) . 2_764 ? 
Mn1 O2 Mn1 144.44(13) . 2_764 ? 
Fe1 O2 Mn1 0.0 2_764 2_764 ? 
Fe1 O2 Y1 97.18(9) . 2_664 ? 
Mn1 O2 Y1 97.18(9) . 2_664 ? 
Fe1 O2 Y1 118.36(11) 2_764 2_664 ? 
Mn1 O2 Y1 118.36(11) 2_764 2_664 ? 
Fe1 O2 Y1 85.71(8) . 5_767 ? 
Mn1 O2 Y1 85.71(8) . 5_767 ? 
Fe1 O2 Y1 86.79(8) 2_764 5_767 ? 
Mn1 O2 Y1 86.79(8) 2_764 5_767 ? 
Y1 O2 Y1 103.31(9) 2_664 5_767 ? 
Fe1 O2 Y1 92.35(9) . 6_657 ? 
Mn1 O2 Y1 92.35(9) . 6_657 ? 
Fe1 O2 Y1 79.50(8) 2_764 6_657 ? 
Mn1 O2 Y1 79.50(8) 2_764 6_657 ? 
Y1 O2 Y1 103.15(8) 2_664 6_657 ? 
Y1 O2 Y1 153.51(10) 5_767 6_657 ? 
Fe1 O1 Mn1 0.0 . . ? 
Fe1 O1 Fe1 143.23(19) . 3_757 ? 
Mn1 O1 Fe1 143.23(19) . 3_757 ? 
Fe1 O1 Mn1 143.23(19) . 3_757 ? 
Mn1 O1 Mn1 143.23(19) . 3_757 ? 
Fe1 O1 Mn1 0.0 3_757 3_757 ? 
Fe1 O1 Y1 104.57(10) . 2_665 ? 
Mn1 O1 Y1 104.57(10) . 2_665 ? 
Fe1 O1 Y1 104.57(10) 3_757 2_665 ? 
Mn1 O1 Y1 104.57(10) 3_757 2_665 ? 
Fe1 O1 Y1 90.99(10) . 5_767 ? 
Mn1 O1 Y1 90.99(10) . 5_767 ? 
Fe1 O1 Y1 90.99(10) 3_757 5_767 ? 
Mn1 O1 Y1 90.99(10) 3_757 5_767 ? 
Y1 O1 Y1 123.97(15) 2_665 5_767 ? 
O1 Y1 O2 101.95(9) 2_664 8_756 ? 
O1 Y1 O2 101.95(9) 2_664 2_665 ? 
O2 Y1 O2 79.45(12) 8_756 2_665 ? 
O1 Y1 O1 89.71(8) 2_664 5_767 ? 
O2 Y1 O1 137.89(6) 8_756 5_767 ? 
O2 Y1 O1 137.89(6) 2_665 5_767 ? 
O1 Y1 O2 137.21(7) 2_664 5_767 ? 
O2 Y1 O2 118.62(5) 8_756 5_767 ? 
O2 Y1 O2 74.57(6) 2_665 5_767 ? 
O1 Y1 O2 69.82(8) 5_767 5_767 ? 
O1 Y1 O2 137.21(7) 2_664 3_747 ? 
O2 Y1 O2 74.57(6) 8_756 3_747 ? 
O2 Y1 O2 118.62(5) 2_665 3_747 ? 
O1 Y1 O2 69.82(8) 5_767 3_747 ? 
O2 Y1 O2 71.33(11) 5_767 3_747 ? 
O1 Y1 O2 69.88(6) 2_664 4_456 ? 
O2 Y1 O2 76.85(9) 8_756 4_456 ? 
O2 Y1 O2 152.47(6) 2_665 4_456 ? 
O1 Y1 O2 69.47(6) 5_767 4_456 ? 
O2 Y1 O2 129.71(4) 5_767 4_456 ? 
O2 Y1 O2 67.82(4) 3_747 4_456 ? 
O1 Y1 O2 69.88(6) 2_664 6_557 ? 
O2 Y1 O2 152.47(6) 8_756 6_557 ? 
O2 Y1 O2 76.85(9) 2_665 6_557 ? 
O1 Y1 O2 69.47(6) 5_767 6_557 ? 
O2 Y1 O2 67.82(4) 5_767 6_557 ? 
O2 Y1 O2 129.71(4) 3_747 6_557 ? 
O2 Y1 O2 121.33(10) 4_456 6_557 ? 
O1 Y1 Mn1 101.50(7) 2_664 . ? 
O2 Y1 Mn1 156.46(6) 8_756 . ? 
O2 Y1 Mn1 97.68(6) 2_665 . ? 
O1 Y1 Mn1 40.21(3) 5_767 . ? 
O2 Y1 Mn1 39.62(5) 5_767 . ? 
O2 Y1 Mn1 86.80(6) 3_747 . ? 
O2 Y1 Mn1 109.63(5) 4_456 . ? 
O2 Y1 Mn1 42.92(5) 6_557 . ? 
O1 Y1 Fe1 101.50(7) 2_664 . ? 
O2 Y1 Fe1 156.46(6) 8_756 . ? 
O2 Y1 Fe1 97.68(6) 2_665 . ? 
O1 Y1 Fe1 40.21(3) 5_767 . ? 
O2 Y1 Fe1 39.62(5) 5_767 . ? 
O2 Y1 Fe1 86.80(6) 3_747 . ? 
O2 Y1 Fe1 109.63(5) 4_456 . ? 
O2 Y1 Fe1 42.92(5) 6_557 . ? 
Mn1 Y1 Fe1 0.0 . . ? 
O1 Y1 Fe1 101.50(7) 2_664 3_747 ? 
O2 Y1 Fe1 97.68(6) 8_756 3_747 ? 
O2 Y1 Fe1 156.46(6) 2_665 3_747 ? 
O1 Y1 Fe1 40.21(3) 5_767 3_747 ? 
O2 Y1 Fe1 86.80(6) 5_767 3_747 ? 
O2 Y1 Fe1 39.62(5) 3_747 3_747 ? 
O2 Y1 Fe1 42.92(5) 4_456 3_747 ? 
O2 Y1 Fe1 109.63(5) 6_557 3_747 ? 
Mn1 Y1 Fe1 75.569(15) . 3_747 ? 
Fe1 Y1 Fe1 75.569(15) . 3_747 ? 
O1 Y1 Mn1 101.50(7) 2_664 3_747 ? 
O2 Y1 Mn1 97.68(6) 8_756 3_747 ? 
O2 Y1 Mn1 156.46(6) 2_665 3_747 ? 
O1 Y1 Mn1 40.21(3) 5_767 3_747 ? 
O2 Y1 Mn1 86.80(6) 5_767 3_747 ? 
O2 Y1 Mn1 39.62(5) 3_747 3_747 ? 
O2 Y1 Mn1 42.92(5) 4_456 3_747 ? 
O2 Y1 Mn1 109.63(5) 6_557 3_747 ? 
Mn1 Y1 Mn1 75.569(15) . 3_747 ? 
Fe1 Y1 Mn1 75.569(15) . 3_747 ? 
Fe1 Y1 Mn1 0.0 3_747 3_747 ? 
O2 Mn1 O2 180.000(1) . 5_767 ? 
O2 Mn1 O1 91.05(12) . 5_767 ? 
O2 Mn1 O1 88.95(12) 5_767 5_767 ? 
O2 Mn1 O1 88.95(12) . . ? 
O2 Mn1 O1 91.05(12) 5_767 . ? 
O1 Mn1 O1 180.000(1) 5_767 . ? 
O2 Mn1 O2 90.82(4) . 6_557 ? 
O2 Mn1 O2 89.18(4) 5_767 6_557 ? 
O1 Mn1 O2 87.05(12) 5_767 6_557 ? 
O1 Mn1 O2 92.95(12) . 6_557 ? 
O2 Mn1 O2 89.18(4) . 2_765 ? 
O2 Mn1 O2 90.82(4) 5_767 2_765 ? 
O1 Mn1 O2 92.95(12) 5_767 2_765 ? 
O1 Mn1 O2 87.05(12) . 2_765 ? 
O2 Mn1 O2 180.0 6_557 2_765 ? 
O2 Mn1 Y1 54.66(7) . 5_767 ? 
O2 Mn1 Y1 125.34(7) 5_767 5_767 ? 
O1 Mn1 Y1 131.20(10) 5_767 5_767 ? 
O1 Mn1 Y1 48.80(10) . 5_767 ? 
O2 Mn1 Y1 122.42(7) 6_557 5_767 ? 
O2 Mn1 Y1 57.58(7) 2_765 5_767 ? 
O2 Mn1 Y1 125.34(7) . . ? 
O2 Mn1 Y1 54.66(7) 5_767 . ? 
O1 Mn1 Y1 48.80(10) 5_767 . ? 
O1 Mn1 Y1 131.20(10) . . ? 
O2 Mn1 Y1 57.58(7) 6_557 . ? 
O2 Mn1 Y1 122.42(7) 2_765 . ? 
Y1 Mn1 Y1 180.0 5_767 . ? 
O2 Mn1 Y1 45.29(7) . 2_664 ? 
O2 Mn1 Y1 134.71(7) 5_767 2_664 ? 
O1 Mn1 Y1 107.90(10) 5_767 2_664 ? 
O1 Mn1 Y1 72.10(10) . 2_664 ? 
O2 Mn1 Y1 51.63(6) 6_557 2_664 ? 
O2 Mn1 Y1 128.37(6) 2_765 2_664 ? 
Y1 Mn1 Y1 73.891(11) 5_767 2_664 ? 
Y1 Mn1 Y1 106.109(11) . 2_664 ? 
O2 Mn1 Y1 134.71(7) . 6_658 ? 
O2 Mn1 Y1 45.29(7) 5_767 6_658 ? 
O1 Mn1 Y1 72.10(10) 5_767 6_658 ? 
O1 Mn1 Y1 107.90(10) . 6_658 ? 
O2 Mn1 Y1 128.37(6) 6_557 6_658 ? 
O2 Mn1 Y1 51.63(6) 2_765 6_658 ? 
Y1 Mn1 Y1 106.109(11) 5_767 6_658 ? 
Y1 Mn1 Y1 73.891(11) . 6_658 ? 
Y1 Mn1 Y1 180.0 2_664 6_658 ? 
O2 Mn1 Y1 51.81(7) . 6_657 ? 
O2 Mn1 Y1 128.19(7) 5_767 6_657 ? 
O1 Mn1 Y1 40.50(10) 5_767 6_657 ? 
O1 Mn1 Y1 139.50(10) . 6_657 ? 
O2 Mn1 Y1 79.67(7) 6_557 6_657 ? 
O2 Mn1 Y1 100.33(7) 2_765 6_657 ? 
Y1 Mn1 Y1 102.498(11) 5_767 6_657 ? 
Y1 Mn1 Y1 77.502(11) . 6_657 ? 
Y1 Mn1 Y1 72.314(10) 2_664 6_657 ? 
Y1 Mn1 Y1 107.686(10) 6_658 6_657 ? 
O2 Mn1 Y1 128.19(7) . 2_665 ? 
O2 Mn1 Y1 51.81(7) 5_767 2_665 ? 
O1 Mn1 Y1 139.50(10) 5_767 2_665 ? 
O1 Mn1 Y1 40.50(10) . 2_665 ? 
O2 Mn1 Y1 100.33(7) 6_557 2_665 ? 
O2 Mn1 Y1 79.67(7) 2_765 2_665 ? 
Y1 Mn1 Y1 77.502(11) 5_767 2_665 ? 
Y1 Mn1 Y1 102.498(11) . 2_665 ? 
Y1 Mn1 Y1 107.686(11) 2_664 2_665 ? 
Y1 Mn1 Y1 72.314(11) 6_658 2_665 ? 
Y1 Mn1 Y1 180.0 6_657 2_665 ? 
O2 Fe1 O2 180.000(1) . 5_767 ? 
O2 Fe1 O1 91.05(12) . 5_767 ? 
O2 Fe1 O1 88.95(12) 5_767 5_767 ? 
O2 Fe1 O1 88.95(12) . . ? 
O2 Fe1 O1 91.05(12) 5_767 . ? 
O1 Fe1 O1 180.000(1) 5_767 . ? 
O2 Fe1 O2 90.82(4) . 6_557 ? 
O2 Fe1 O2 89.18(4) 5_767 6_557 ? 
O1 Fe1 O2 87.05(12) 5_767 6_557 ? 
O1 Fe1 O2 92.95(12) . 6_557 ? 
O2 Fe1 O2 89.18(4) . 2_765 ? 
O2 Fe1 O2 90.82(4) 5_767 2_765 ? 
O1 Fe1 O2 92.95(12) 5_767 2_765 ? 
O1 Fe1 O2 87.05(12) . 2_765 ? 
O2 Fe1 O2 180.0 6_557 2_765 ? 
O2 Fe1 Y1 54.66(7) . 5_767 ? 
O2 Fe1 Y1 125.34(7) 5_767 5_767 ? 
O1 Fe1 Y1 131.20(10) 5_767 5_767 ? 
O1 Fe1 Y1 48.80(10) . 5_767 ? 
O2 Fe1 Y1 122.42(7) 6_557 5_767 ? 
O2 Fe1 Y1 57.58(7) 2_765 5_767 ? 
O2 Fe1 Y1 125.34(7) . . ? 
O2 Fe1 Y1 54.66(7) 5_767 . ? 
O1 Fe1 Y1 48.80(10) 5_767 . ? 
O1 Fe1 Y1 131.20(10) . . ? 
O2 Fe1 Y1 57.58(7) 6_557 . ? 
O2 Fe1 Y1 122.42(7) 2_765 . ? 
Y1 Fe1 Y1 180.0 5_767 . ? 
O2 Fe1 Y1 45.29(7) . 2_664 ? 
O2 Fe1 Y1 134.71(7) 5_767 2_664 ? 
O1 Fe1 Y1 107.90(10) 5_767 2_664 ? 
O1 Fe1 Y1 72.10(10) . 2_664 ? 
O2 Fe1 Y1 51.63(6) 6_557 2_664 ? 
O2 Fe1 Y1 128.37(6) 2_765 2_664 ? 
Y1 Fe1 Y1 73.891(11) 5_767 2_664 ? 
Y1 Fe1 Y1 106.109(11) . 2_664 ? 
O2 Fe1 Y1 134.71(7) . 6_658 ? 
O2 Fe1 Y1 45.29(7) 5_767 6_658 ? 
O1 Fe1 Y1 72.10(10) 5_767 6_658 ? 
O1 Fe1 Y1 107.90(10) . 6_658 ? 
O2 Fe1 Y1 128.37(6) 6_557 6_658 ? 
O2 Fe1 Y1 51.63(6) 2_765 6_658 ? 
Y1 Fe1 Y1 106.109(11) 5_767 6_658 ? 
Y1 Fe1 Y1 73.891(11) . 6_658 ? 
Y1 Fe1 Y1 180.0 2_664 6_658 ? 
O2 Fe1 Y1 51.81(7) . 6_657 ? 
O2 Fe1 Y1 128.19(7) 5_767 6_657 ? 
O1 Fe1 Y1 40.50(10) 5_767 6_657 ? 
O1 Fe1 Y1 139.50(10) . 6_657 ? 
O2 Fe1 Y1 79.67(7) 6_557 6_657 ? 
O2 Fe1 Y1 100.33(7) 2_765 6_657 ? 
Y1 Fe1 Y1 102.498(11) 5_767 6_657 ? 
Y1 Fe1 Y1 77.502(11) . 6_657 ? 
Y1 Fe1 Y1 72.314(10) 2_664 6_657 ? 
Y1 Fe1 Y1 107.686(10) 6_658 6_657 ? 
O2 Fe1 Y1 128.19(7) . 2_665 ? 
O2 Fe1 Y1 51.81(7) 5_767 2_665 ? 
O1 Fe1 Y1 139.50(10) 5_767 2_665 ? 
O1 Fe1 Y1 40.50(10) . 2_665 ? 
O2 Fe1 Y1 100.33(7) 6_557 2_665 ? 
O2 Fe1 Y1 79.67(7) 2_765 2_665 ? 
Y1 Fe1 Y1 77.502(11) 5_767 2_665 ? 
Y1 Fe1 Y1 102.498(11) . 2_665 ? 
Y1 Fe1 Y1 107.686(11) 2_664 2_665 ? 
Y1 Fe1 Y1 72.314(11) 6_658 2_665 ? 
Y1 Fe1 Y1 180.0 6_657 2_665 ? 
 
loop_ 
 _geom_torsion_atom_site_label_1 
 _geom_torsion_atom_site_label_2 
 _geom_torsion_atom_site_label_3 
 _geom_torsion_atom_site_label_4 
 _geom_torsion 
 _geom_torsion_site_symmetry_1 
 _geom_torsion_site_symmetry_2 
 _geom_torsion_site_symmetry_3 
 _geom_torsion_site_symmetry_4 
 _geom_torsion_publ_flag 
Fe1 O2 Mn1 O2 0(100) . . . 5_767 ? 
Fe1 O2 Mn1 O2 -147(100) 2_764 . . 5_767 ? 
Mn1 O2 Mn1 O2 -147(100) 2_764 . . 5_767 ? 
Y1 O2 Mn1 O2 31(100) 2_664 . . 5_767 ? 
Y1 O2 Mn1 O2 134(100) 5_767 . . 5_767 ? 
Y1 O2 Mn1 O2 -72(100) 6_657 . . 5_767 ? 
Fe1 O2 Mn1 O1 0(100) . . . 5_767 ? 
Fe1 O2 Mn1 O1 -64.2(2) 2_764 . . 5_767 ? 
Mn1 O2 Mn1 O1 -64.2(2) 2_764 . . 5_767 ? 
Y1 O2 Mn1 O1 114.49(12) 2_664 . . 5_767 ? 
Y1 O2 Mn1 O1 -142.62(11) 5_767 . . 5_767 ? 
Y1 O2 Mn1 O1 10.91(11) 6_657 . . 5_767 ? 
Fe1 O2 Mn1 O1 0(100) . . . . ? 
Fe1 O2 Mn1 O1 115.8(2) 2_764 . . . ? 
Mn1 O2 Mn1 O1 115.8(2) 2_764 . . . ? 
Y1 O2 Mn1 O1 -65.51(12) 2_664 . . . ? 
Y1 O2 Mn1 O1 37.38(11) 5_767 . . . ? 
Y1 O2 Mn1 O1 -169.09(11) 6_657 . . . ? 
Fe1 O2 Mn1 O2 0(100) . . . 6_557 ? 
Fe1 O2 Mn1 O2 -151.30(17) 2_764 . . 6_557 ? 
Mn1 O2 Mn1 O2 -151.30(17) 2_764 . . 6_557 ? 
Y1 O2 Mn1 O2 27.43(13) 2_664 . . 6_557 ? 
Y1 O2 Mn1 O2 130.32(4) 5_767 . . 6_557 ? 
Y1 O2 Mn1 O2 -76.14(11) 6_657 . . 6_557 ? 
Fe1 O2 Mn1 O2 0(100) . . . 2_765 ? 
Fe1 O2 Mn1 O2 28.70(17) 2_764 . . 2_765 ? 
Mn1 O2 Mn1 O2 28.70(17) 2_764 . . 2_765 ? 
Y1 O2 Mn1 O2 -152.57(13) 2_664 . . 2_765 ? 
Y1 O2 Mn1 O2 -49.68(4) 5_767 . . 2_765 ? 
Y1 O2 Mn1 O2 103.86(11) 6_657 . . 2_765 ? 
Fe1 O2 Mn1 Y1 0(100) . . . 5_767 ? 
Fe1 O2 Mn1 Y1 78.4(2) 2_764 . . 5_767 ? 
Mn1 O2 Mn1 Y1 78.4(2) 2_764 . . 5_767 ? 
Y1 O2 Mn1 Y1 -102.90(10) 2_664 . . 5_767 ? 
Y1 O2 Mn1 Y1 153.53(10) 6_657 . . 5_767 ? 
Fe1 O2 Mn1 Y1 0(29) . . . . ? 
Fe1 O2 Mn1 Y1 -101.6(2) 2_764 . . . ? 
Mn1 O2 Mn1 Y1 -101.6(2) 2_764 . . . ? 
Y1 O2 Mn1 Y1 77.10(10) 2_664 . . . ? 
Y1 O2 Mn1 Y1 180.0 5_767 . . . ? 
Y1 O2 Mn1 Y1 -26.47(10) 6_657 . . . ? 
Fe1 O2 Mn1 Y1 0(100) . . . 2_664 ? 
Fe1 O2 Mn1 Y1 -178.7(3) 2_764 . . 2_664 ? 
Mn1 O2 Mn1 Y1 -178.7(3) 2_764 . . 2_664 ? 
Y1 O2 Mn1 Y1 102.90(10) 5_767 . . 2_664 ? 
Y1 O2 Mn1 Y1 -103.57(9) 6_657 . . 2_664 ? 
Fe1 O2 Mn1 Y1 0(100) . . . 6_658 ? 
Fe1 O2 Mn1 Y1 1.3(3) 2_764 . . 6_658 ? 
Mn1 O2 Mn1 Y1 1.3(3) 2_764 . . 6_658 ? 
Y1 O2 Mn1 Y1 180.0 2_664 . . 6_658 ? 
Y1 O2 Mn1 Y1 -77.10(10) 5_767 . . 6_658 ? 
Y1 O2 Mn1 Y1 76.43(9) 6_657 . . 6_658 ? 
Fe1 O2 Mn1 Y1 0(100) . . . 6_657 ? 
Fe1 O2 Mn1 Y1 -75.2(2) 2_764 . . 6_657 ? 
Mn1 O2 Mn1 Y1 -75.2(2) 2_764 . . 6_657 ? 
Y1 O2 Mn1 Y1 103.57(10) 2_664 . . 6_657 ? 
Y1 O2 Mn1 Y1 -153.53(10) 5_767 . . 6_657 ? 
Fe1 O2 Mn1 Y1 0(100) . . . 2_665 ? 
Fe1 O2 Mn1 Y1 104.8(2) 2_764 . . 2_665 ? 
Mn1 O2 Mn1 Y1 104.8(2) 2_764 . . 2_665 ? 
Y1 O2 Mn1 Y1 -76.43(9) 2_664 . . 2_665 ? 
Y1 O2 Mn1 Y1 26.47(10) 5_767 . . 2_665 ? 
Y1 O2 Mn1 Y1 180.0 6_657 . . 2_665 ? 
Fe1 O1 Mn1 O2 0(100) . . . . ? 
Fe1 O1 Mn1 O2 51.8(3) 3_757 . . . ? 
Mn1 O1 Mn1 O2 51.8(3) 3_757 . . . ? 
Y1 O1 Mn1 O2 -166.75(13) 2_665 . . . ? 
Y1 O1 Mn1 O2 -41.17(10) 5_767 . . . ? 
Fe1 O1 Mn1 O2 0(100) . . . 5_767 ? 
Fe1 O1 Mn1 O2 -128.2(3) 3_757 . . 5_767 ? 
Mn1 O1 Mn1 O2 -128.2(3) 3_757 . . 5_767 ? 
Y1 O1 Mn1 O2 13.25(13) 2_665 . . 5_767 ? 
Y1 O1 Mn1 O2 138.83(10) 5_767 . . 5_767 ? 
Fe1 O1 Mn1 O1 0(100) . . . 5_767 ? 
Fe1 O1 Mn1 O1 -71(100) 3_757 . . 5_767 ? 
Mn1 O1 Mn1 O1 -71(100) 3_757 . . 5_767 ? 
Y1 O1 Mn1 O1 71(100) 2_665 . . 5_767 ? 
Y1 O1 Mn1 O1 -164(100) 5_767 . . 5_767 ? 
Fe1 O1 Mn1 O2 0(100) . . . 6_557 ? 
Fe1 O1 Mn1 O2 -38.9(3) 3_757 . . 6_557 ? 
Mn1 O1 Mn1 O2 -38.9(3) 3_757 . . 6_557 ? 
Y1 O1 Mn1 O2 102.48(13) 2_665 . . 6_557 ? 
Y1 O1 Mn1 O2 -131.93(10) 5_767 . . 6_557 ? 
Fe1 O1 Mn1 O2 0(100) . . . 2_765 ? 
Fe1 O1 Mn1 O2 141.1(3) 3_757 . . 2_765 ? 
Mn1 O1 Mn1 O2 141.1(3) 3_757 . . 2_765 ? 
Y1 O1 Mn1 O2 -77.52(13) 2_665 . . 2_765 ? 
Y1 O1 Mn1 O2 48.07(10) 5_767 . . 2_765 ? 
Fe1 O1 Mn1 Y1 0(100) . . . 5_767 ? 
Fe1 O1 Mn1 Y1 93.0(3) 3_757 . . 5_767 ? 
Mn1 O1 Mn1 Y1 93.0(3) 3_757 . . 5_767 ? 
Y1 O1 Mn1 Y1 -125.59(17) 2_665 . . 5_767 ? 
Fe1 O1 Mn1 Y1 0(23) . . . . ? 
Fe1 O1 Mn1 Y1 -87.0(3) 3_757 . . . ? 
Mn1 O1 Mn1 Y1 -87.0(3) 3_757 . . . ? 
Y1 O1 Mn1 Y1 54.41(17) 2_665 . . . ? 
Y1 O1 Mn1 Y1 180.0 5_767 . . . ? 
Fe1 O1 Mn1 Y1 0(100) . . . 2_664 ? 
Fe1 O1 Mn1 Y1 9.0(3) 3_757 . . 2_664 ? 
Mn1 O1 Mn1 Y1 9.0(3) 3_757 . . 2_664 ? 
Y1 O1 Mn1 Y1 150.43(14) 2_665 . . 2_664 ? 
Y1 O1 Mn1 Y1 -83.99(9) 5_767 . . 2_664 ? 
Fe1 O1 Mn1 Y1 0(100) . . . 6_658 ? 
Fe1 O1 Mn1 Y1 -171.0(3) 3_757 . . 6_658 ? 
Mn1 O1 Mn1 Y1 -171.0(3) 3_757 . . 6_658 ? 
Y1 O1 Mn1 Y1 -29.57(14) 2_665 . . 6_658 ? 
Y1 O1 Mn1 Y1 96.01(9) 5_767 . . 6_658 ? 
Fe1 O1 Mn1 Y1 0(100) . . . 6_657 ? 
Fe1 O1 Mn1 Y1 38.6(4) 3_757 . . 6_657 ? 
Mn1 O1 Mn1 Y1 38.6(4) 3_757 . . 6_657 ? 
Y1 O1 Mn1 Y1 180.0 2_665 . . 6_657 ? 
Y1 O1 Mn1 Y1 -54.41(17) 5_767 . . 6_657 ? 
Fe1 O1 Mn1 Y1 0(100) . . . 2_665 ? 
Fe1 O1 Mn1 Y1 -141.4(4) 3_757 . . 2_665 ? 
Mn1 O1 Mn1 Y1 -141.4(4) 3_757 . . 2_665 ? 
Y1 O1 Mn1 Y1 125.59(17) 5_767 . . 2_665 ? 
O1 Y1 Mn1 O2 -21.81(10) 2_664 . . . ? 
O2 Y1 Mn1 O2 153.1(2) 8_756 . . . ? 
O2 Y1 Mn1 O2 -125.73(9) 2_665 . . . ? 
O1 Y1 Mn1 O2 53.78(15) 5_767 . . . ? 
O2 Y1 Mn1 O2 180.0 5_767 . . . ? 
O2 Y1 Mn1 O2 115.80(12) 3_747 . . . ? 
O2 Y1 Mn1 O2 50.73(12) 4_456 . . . ? 
O2 Y1 Mn1 O2 -64.56(6) 6_557 . . . ? 
Fe1 Y1 Mn1 O2 0(44) . . . . ? 
Fe1 Y1 Mn1 O2 77.27(9) 3_747 . . . ? 
Mn1 Y1 Mn1 O2 77.27(9) 3_747 . . . ? 
O1 Y1 Mn1 O2 158.19(10) 2_664 . . 5_767 ? 
O2 Y1 Mn1 O2 -26.9(2) 8_756 . . 5_767 ? 
O2 Y1 Mn1 O2 54.27(9) 2_665 . . 5_767 ? 
O1 Y1 Mn1 O2 -126.22(15) 5_767 . . 5_767 ? 
O2 Y1 Mn1 O2 -64.20(12) 3_747 . . 5_767 ? 
O2 Y1 Mn1 O2 -129.27(12) 4_456 . . 5_767 ? 
O2 Y1 Mn1 O2 115.44(6) 6_557 . . 5_767 ? 
Fe1 Y1 Mn1 O2 0(44) . . . 5_767 ? 
Fe1 Y1 Mn1 O2 -102.73(9) 3_747 . . 5_767 ? 
Mn1 Y1 Mn1 O2 -102.73(9) 3_747 . . 5_767 ? 
O1 Y1 Mn1 O1 -75.59(11) 2_664 . . 5_767 ? 
O2 Y1 Mn1 O1 99.30(19) 8_756 . . 5_767 ? 
O2 Y1 Mn1 O1 -179.51(14) 2_665 . . 5_767 ? 
O2 Y1 Mn1 O1 126.22(15) 5_767 . . 5_767 ? 
O2 Y1 Mn1 O1 62.02(14) 3_747 . . 5_767 ? 
O2 Y1 Mn1 O1 -3.05(14) 4_456 . . 5_767 ? 
O2 Y1 Mn1 O1 -118.34(15) 6_557 . . 5_767 ? 
Fe1 Y1 Mn1 O1 0(70) . . . 5_767 ? 
Fe1 Y1 Mn1 O1 23.49(13) 3_747 . . 5_767 ? 
Mn1 Y1 Mn1 O1 23.49(13) 3_747 . . 5_767 ? 
O1 Y1 Mn1 O1 104.41(11) 2_664 . . . ? 
O2 Y1 Mn1 O1 -80.70(19) 8_756 . . . ? 
O2 Y1 Mn1 O1 0.49(14) 2_665 . . . ? 
O1 Y1 Mn1 O1 180.0 5_767 . . . ? 
O2 Y1 Mn1 O1 -53.78(15) 5_767 . . . ? 
O2 Y1 Mn1 O1 -117.98(13) 3_747 . . . ? 
O2 Y1 Mn1 O1 176.95(14) 4_456 . . . ? 
O2 Y1 Mn1 O1 61.66(15) 6_557 . . . ? 
Fe1 Y1 Mn1 O1 0(18) . . . . ? 
Fe1 Y1 Mn1 O1 -156.51(13) 3_747 . . . ? 
Mn1 Y1 Mn1 O1 -156.51(13) 3_747 . . . ? 
O1 Y1 Mn1 O2 42.75(9) 2_664 . . 6_557 ? 
O2 Y1 Mn1 O2 -142.36(17) 8_756 . . 6_557 ? 
O2 Y1 Mn1 O2 -61.17(12) 2_665 . . 6_557 ? 
O1 Y1 Mn1 O2 118.34(15) 5_767 . . 6_557 ? 
O2 Y1 Mn1 O2 -115.44(6) 5_767 . . 6_557 ? 
O2 Y1 Mn1 O2 -179.64(12) 3_747 . . 6_557 ? 
O2 Y1 Mn1 O2 115.29(12) 4_456 . . 6_557 ? 
Fe1 Y1 Mn1 O2 0(12) . . . 6_557 ? 
Fe1 Y1 Mn1 O2 141.83(8) 3_747 . . 6_557 ? 
Mn1 Y1 Mn1 O2 141.83(8) 3_747 . . 6_557 ? 
O1 Y1 Mn1 O2 -137.25(9) 2_664 . . 2_765 ? 
O2 Y1 Mn1 O2 37.64(17) 8_756 . . 2_765 ? 
O2 Y1 Mn1 O2 118.83(12) 2_665 . . 2_765 ? 
O1 Y1 Mn1 O2 -61.66(15) 5_767 . . 2_765 ? 
O2 Y1 Mn1 O2 64.56(6) 5_767 . . 2_765 ? 
O2 Y1 Mn1 O2 0.36(12) 3_747 . . 2_765 ? 
O2 Y1 Mn1 O2 -64.71(12) 4_456 . . 2_765 ? 
O2 Y1 Mn1 O2 180.0 6_557 . . 2_765 ? 
Fe1 Y1 Mn1 O2 0(75) . . . 2_765 ? 
Fe1 Y1 Mn1 O2 -38.17(8) 3_747 . . 2_765 ? 
Mn1 Y1 Mn1 O2 -38.17(8) 3_747 . . 2_765 ? 
O1 Y1 Mn1 Y1 78(17) 2_664 . . 5_767 ? 
O2 Y1 Mn1 Y1 -107(17) 8_756 . . 5_767 ? 
O2 Y1 Mn1 Y1 -26(17) 2_665 . . 5_767 ? 
O1 Y1 Mn1 Y1 154(17) 5_767 . . 5_767 ? 
O2 Y1 Mn1 Y1 -80(17) 5_767 . . 5_767 ? 
O2 Y1 Mn1 Y1 -144(17) 3_747 . . 5_767 ? 
O2 Y1 Mn1 Y1 151(17) 4_456 . . 5_767 ? 
O2 Y1 Mn1 Y1 35(17) 6_557 . . 5_767 ? 
Fe1 Y1 Mn1 Y1 0(67) . . . 5_767 ? 
Fe1 Y1 Mn1 Y1 177(17) 3_747 . . 5_767 ? 
Mn1 Y1 Mn1 Y1 177(17) 3_747 . . 5_767 ? 
O1 Y1 Mn1 Y1 24.34(6) 2_664 . . 2_664 ? 
O2 Y1 Mn1 Y1 -160.78(16) 8_756 . . 2_664 ? 
O2 Y1 Mn1 Y1 -79.59(6) 2_665 . . 2_664 ? 
O1 Y1 Mn1 Y1 99.93(13) 5_767 . . 2_664 ? 
O2 Y1 Mn1 Y1 -133.85(9) 5_767 . . 2_664 ? 
O2 Y1 Mn1 Y1 161.95(5) 3_747 . . 2_664 ? 
O2 Y1 Mn1 Y1 96.87(5) 4_456 . . 2_664 ? 
O2 Y1 Mn1 Y1 -18.41(8) 6_557 . . 2_664 ? 
Fe1 Y1 Mn1 Y1 0(21) . . . 2_664 ? 
Fe1 Y1 Mn1 Y1 123.413(5) 3_747 . . 2_664 ? 
Mn1 Y1 Mn1 Y1 123.413(5) 3_747 . . 2_664 ? 
O1 Y1 Mn1 Y1 -155.66(6) 2_664 . . 6_658 ? 
O2 Y1 Mn1 Y1 19.22(16) 8_756 . . 6_658 ? 
O2 Y1 Mn1 Y1 100.41(6) 2_665 . . 6_658 ? 
O1 Y1 Mn1 Y1 -80.07(13) 5_767 . . 6_658 ? 
O2 Y1 Mn1 Y1 46.15(9) 5_767 . . 6_658 ? 
O2 Y1 Mn1 Y1 -18.05(5) 3_747 . . 6_658 ? 
O2 Y1 Mn1 Y1 -83.13(5) 4_456 . . 6_658 ? 
O2 Y1 Mn1 Y1 161.59(8) 6_557 . . 6_658 ? 
Fe1 Y1 Mn1 Y1 0(66) . . . 6_658 ? 
Fe1 Y1 Mn1 Y1 -56.587(5) 3_747 . . 6_658 ? 
Mn1 Y1 Mn1 Y1 -56.587(5) 3_747 . . 6_658 ? 
O1 Y1 Mn1 Y1 -42.84(6) 2_664 . . 6_657 ? 
O2 Y1 Mn1 Y1 132.05(15) 8_756 . . 6_657 ? 
O2 Y1 Mn1 Y1 -146.76(6) 2_665 . . 6_657 ? 
O1 Y1 Mn1 Y1 32.75(13) 5_767 . . 6_657 ? 
O2 Y1 Mn1 Y1 158.97(9) 5_767 . . 6_657 ? 
O2 Y1 Mn1 Y1 94.78(5) 3_747 . . 6_657 ? 
O2 Y1 Mn1 Y1 29.70(5) 4_456 . . 6_657 ? 
O2 Y1 Mn1 Y1 -85.59(8) 6_557 . . 6_657 ? 
Fe1 Y1 Mn1 Y1 0(54) . . . 6_657 ? 
Fe1 Y1 Mn1 Y1 56.238(6) 3_747 . . 6_657 ? 
Mn1 Y1 Mn1 Y1 56.238(6) 3_747 . . 6_657 ? 
O1 Y1 Mn1 Y1 137.16(6) 2_664 . . 2_665 ? 
O2 Y1 Mn1 Y1 -47.95(15) 8_756 . . 2_665 ? 
O2 Y1 Mn1 Y1 33.24(6) 2_665 . . 2_665 ? 
O1 Y1 Mn1 Y1 -147.25(13) 5_767 . . 2_665 ? 
O2 Y1 Mn1 Y1 -21.03(9) 5_767 . . 2_665 ? 
O2 Y1 Mn1 Y1 -85.22(5) 3_747 . . 2_665 ? 
O2 Y1 Mn1 Y1 -150.30(5) 4_456 . . 2_665 ? 
O2 Y1 Mn1 Y1 94.41(8) 6_557 . . 2_665 ? 
Fe1 Y1 Mn1 Y1 0(34) . . . 2_665 ? 
Fe1 Y1 Mn1 Y1 -123.762(6) 3_747 . . 2_665 ? 
Mn1 Y1 Mn1 Y1 -123.762(6) 3_747 . . 2_665 ? 
Mn1 O2 Fe1 O2 0(100) . . . 5_767 ? 
Fe1 O2 Fe1 O2 -147(100) 2_764 . . 5_767 ? 
Mn1 O2 Fe1 O2 -147(100) 2_764 . . 5_767 ? 
Y1 O2 Fe1 O2 31(100) 2_664 . . 5_767 ? 
Y1 O2 Fe1 O2 134(100) 5_767 . . 5_767 ? 
Y1 O2 Fe1 O2 -72(100) 6_657 . . 5_767 ? 
Mn1 O2 Fe1 O1 0(100) . . . 5_767 ? 
Fe1 O2 Fe1 O1 -64.2(2) 2_764 . . 5_767 ? 
Mn1 O2 Fe1 O1 -64.2(2) 2_764 . . 5_767 ? 
Y1 O2 Fe1 O1 114.49(12) 2_664 . . 5_767 ? 
Y1 O2 Fe1 O1 -142.62(11) 5_767 . . 5_767 ? 
Y1 O2 Fe1 O1 10.91(11) 6_657 . . 5_767 ? 
Mn1 O2 Fe1 O1 0(100) . . . . ? 
Fe1 O2 Fe1 O1 115.8(2) 2_764 . . . ? 
Mn1 O2 Fe1 O1 115.8(2) 2_764 . . . ? 
Y1 O2 Fe1 O1 -65.51(12) 2_664 . . . ? 
Y1 O2 Fe1 O1 37.38(11) 5_767 . . . ? 
Y1 O2 Fe1 O1 -169.09(11) 6_657 . . . ? 
Mn1 O2 Fe1 O2 0(100) . . . 6_557 ? 
Fe1 O2 Fe1 O2 -151.30(17) 2_764 . . 6_557 ? 
Mn1 O2 Fe1 O2 -151.30(17) 2_764 . . 6_557 ? 
Y1 O2 Fe1 O2 27.43(13) 2_664 . . 6_557 ? 
Y1 O2 Fe1 O2 130.32(4) 5_767 . . 6_557 ? 
Y1 O2 Fe1 O2 -76.14(11) 6_657 . . 6_557 ? 
Mn1 O2 Fe1 O2 0(100) . . . 2_765 ? 
Fe1 O2 Fe1 O2 28.70(17) 2_764 . . 2_765 ? 
Mn1 O2 Fe1 O2 28.70(17) 2_764 . . 2_765 ? 
Y1 O2 Fe1 O2 -152.57(13) 2_664 . . 2_765 ? 
Y1 O2 Fe1 O2 -49.68(4) 5_767 . . 2_765 ? 
Y1 O2 Fe1 O2 103.86(11) 6_657 . . 2_765 ? 
Mn1 O2 Fe1 Y1 0(100) . . . 5_767 ? 
Fe1 O2 Fe1 Y1 78.4(2) 2_764 . . 5_767 ? 
Mn1 O2 Fe1 Y1 78.4(2) 2_764 . . 5_767 ? 
Y1 O2 Fe1 Y1 -102.90(10) 2_664 . . 5_767 ? 
Y1 O2 Fe1 Y1 153.53(10) 6_657 . . 5_767 ? 
Mn1 O2 Fe1 Y1 0(29) . . . . ? 
Fe1 O2 Fe1 Y1 -101.6(2) 2_764 . . . ? 
Mn1 O2 Fe1 Y1 -101.6(2) 2_764 . . . ? 
Y1 O2 Fe1 Y1 77.10(10) 2_664 . . . ? 
Y1 O2 Fe1 Y1 180.0 5_767 . . . ? 
Y1 O2 Fe1 Y1 -26.47(10) 6_657 . . . ? 
Mn1 O2 Fe1 Y1 0(100) . . . 2_664 ? 
Fe1 O2 Fe1 Y1 -178.7(3) 2_764 . . 2_664 ? 
Mn1 O2 Fe1 Y1 -178.7(3) 2_764 . . 2_664 ? 
Y1 O2 Fe1 Y1 102.90(10) 5_767 . . 2_664 ? 
Y1 O2 Fe1 Y1 -103.57(9) 6_657 . . 2_664 ? 
Mn1 O2 Fe1 Y1 0(100) . . . 6_658 ? 
Fe1 O2 Fe1 Y1 1.3(3) 2_764 . . 6_658 ? 
Mn1 O2 Fe1 Y1 1.3(3) 2_764 . . 6_658 ? 
Y1 O2 Fe1 Y1 180.0 2_664 . . 6_658 ? 
Y1 O2 Fe1 Y1 -77.10(10) 5_767 . . 6_658 ? 
Y1 O2 Fe1 Y1 76.43(9) 6_657 . . 6_658 ? 
Mn1 O2 Fe1 Y1 0(100) . . . 6_657 ? 
Fe1 O2 Fe1 Y1 -75.2(2) 2_764 . . 6_657 ? 
Mn1 O2 Fe1 Y1 -75.2(2) 2_764 . . 6_657 ? 
Y1 O2 Fe1 Y1 103.57(10) 2_664 . . 6_657 ? 
Y1 O2 Fe1 Y1 -153.53(10) 5_767 . . 6_657 ? 
Mn1 O2 Fe1 Y1 0(100) . . . 2_665 ? 
Fe1 O2 Fe1 Y1 104.8(2) 2_764 . . 2_665 ? 
Mn1 O2 Fe1 Y1 104.8(2) 2_764 . . 2_665 ? 
Y1 O2 Fe1 Y1 -76.43(9) 2_664 . . 2_665 ? 
Y1 O2 Fe1 Y1 26.47(10) 5_767 . . 2_665 ? 
Y1 O2 Fe1 Y1 180.0 6_657 . . 2_665 ? 
Mn1 O1 Fe1 O2 0(100) . . . . ? 
Fe1 O1 Fe1 O2 51.8(3) 3_757 . . . ? 
Mn1 O1 Fe1 O2 51.8(3) 3_757 . . . ? 
Y1 O1 Fe1 O2 -166.75(13) 2_665 . . . ? 
Y1 O1 Fe1 O2 -41.17(10) 5_767 . . . ? 
Mn1 O1 Fe1 O2 0(100) . . . 5_767 ? 
Fe1 O1 Fe1 O2 -128.2(3) 3_757 . . 5_767 ? 
Mn1 O1 Fe1 O2 -128.2(3) 3_757 . . 5_767 ? 
Y1 O1 Fe1 O2 13.25(13) 2_665 . . 5_767 ? 
Y1 O1 Fe1 O2 138.83(10) 5_767 . . 5_767 ? 
Mn1 O1 Fe1 O1 0(100) . . . 5_767 ? 
Fe1 O1 Fe1 O1 -71(100) 3_757 . . 5_767 ? 
Mn1 O1 Fe1 O1 -71(100) 3_757 . . 5_767 ? 
Y1 O1 Fe1 O1 71(100) 2_665 . . 5_767 ? 
Y1 O1 Fe1 O1 -164(100) 5_767 . . 5_767 ? 
Mn1 O1 Fe1 O2 0(100) . . . 6_557 ? 
Fe1 O1 Fe1 O2 -38.9(3) 3_757 . . 6_557 ? 
Mn1 O1 Fe1 O2 -38.9(3) 3_757 . . 6_557 ? 
Y1 O1 Fe1 O2 102.48(13) 2_665 . . 6_557 ? 
Y1 O1 Fe1 O2 -131.93(10) 5_767 . . 6_557 ? 
Mn1 O1 Fe1 O2 0(100) . . . 2_765 ? 
Fe1 O1 Fe1 O2 141.1(3) 3_757 . . 2_765 ? 
Mn1 O1 Fe1 O2 141.1(3) 3_757 . . 2_765 ? 
Y1 O1 Fe1 O2 -77.52(13) 2_665 . . 2_765 ? 
Y1 O1 Fe1 O2 48.07(10) 5_767 . . 2_765 ? 
Mn1 O1 Fe1 Y1 0(100) . . . 5_767 ? 
Fe1 O1 Fe1 Y1 93.0(3) 3_757 . . 5_767 ? 
Mn1 O1 Fe1 Y1 93.0(3) 3_757 . . 5_767 ? 
Y1 O1 Fe1 Y1 -125.59(17) 2_665 . . 5_767 ? 
Mn1 O1 Fe1 Y1 0(23) . . . . ? 
Fe1 O1 Fe1 Y1 -87.0(3) 3_757 . . . ? 
Mn1 O1 Fe1 Y1 -87.0(3) 3_757 . . . ? 
Y1 O1 Fe1 Y1 54.41(17) 2_665 . . . ? 
Y1 O1 Fe1 Y1 180.0 5_767 . . . ? 
Mn1 O1 Fe1 Y1 0(100) . . . 2_664 ? 
Fe1 O1 Fe1 Y1 9.0(3) 3_757 . . 2_664 ? 
Mn1 O1 Fe1 Y1 9.0(3) 3_757 . . 2_664 ? 
Y1 O1 Fe1 Y1 150.43(14) 2_665 . . 2_664 ? 
Y1 O1 Fe1 Y1 -83.99(9) 5_767 . . 2_664 ? 
Mn1 O1 Fe1 Y1 0(100) . . . 6_658 ? 
Fe1 O1 Fe1 Y1 -171.0(3) 3_757 . . 6_658 ? 
Mn1 O1 Fe1 Y1 -171.0(3) 3_757 . . 6_658 ? 
Y1 O1 Fe1 Y1 -29.57(14) 2_665 . . 6_658 ? 
Y1 O1 Fe1 Y1 96.01(9) 5_767 . . 6_658 ? 
Mn1 O1 Fe1 Y1 0(100) . . . 6_657 ? 
Fe1 O1 Fe1 Y1 38.6(4) 3_757 . . 6_657 ? 
Mn1 O1 Fe1 Y1 38.6(4) 3_757 . . 6_657 ? 
Y1 O1 Fe1 Y1 180.0 2_665 . . 6_657 ? 
Y1 O1 Fe1 Y1 -54.41(17) 5_767 . . 6_657 ? 
Mn1 O1 Fe1 Y1 0(100) . . . 2_665 ? 
Fe1 O1 Fe1 Y1 -141.4(4) 3_757 . . 2_665 ? 
Mn1 O1 Fe1 Y1 -141.4(4) 3_757 . . 2_665 ? 
Y1 O1 Fe1 Y1 125.59(17) 5_767 . . 2_665 ? 
O1 Y1 Fe1 O2 -21.81(10) 2_664 . . . ? 
O2 Y1 Fe1 O2 153.1(2) 8_756 . . . ? 
O2 Y1 Fe1 O2 -125.73(9) 2_665 . . . ? 
O1 Y1 Fe1 O2 53.78(15) 5_767 . . . ? 
O2 Y1 Fe1 O2 180.0 5_767 . . . ? 
O2 Y1 Fe1 O2 115.80(12) 3_747 . . . ? 
O2 Y1 Fe1 O2 50.73(12) 4_456 . . . ? 
O2 Y1 Fe1 O2 -64.56(6) 6_557 . . . ? 
Mn1 Y1 Fe1 O2 0(44) . . . . ? 
Fe1 Y1 Fe1 O2 77.27(9) 3_747 . . . ? 
Mn1 Y1 Fe1 O2 77.27(9) 3_747 . . . ? 
O1 Y1 Fe1 O2 158.19(10) 2_664 . . 5_767 ? 
O2 Y1 Fe1 O2 -26.9(2) 8_756 . . 5_767 ? 
O2 Y1 Fe1 O2 54.27(9) 2_665 . . 5_767 ? 
O1 Y1 Fe1 O2 -126.22(15) 5_767 . . 5_767 ? 
O2 Y1 Fe1 O2 -64.20(12) 3_747 . . 5_767 ? 
O2 Y1 Fe1 O2 -129.27(12) 4_456 . . 5_767 ? 
O2 Y1 Fe1 O2 115.44(6) 6_557 . . 5_767 ? 
Mn1 Y1 Fe1 O2 0(44) . . . 5_767 ? 
Fe1 Y1 Fe1 O2 -102.73(9) 3_747 . . 5_767 ? 
Mn1 Y1 Fe1 O2 -102.73(9) 3_747 . . 5_767 ? 
O1 Y1 Fe1 O1 -75.59(11) 2_664 . . 5_767 ? 
O2 Y1 Fe1 O1 99.30(19) 8_756 . . 5_767 ? 
O2 Y1 Fe1 O1 -179.51(14) 2_665 . . 5_767 ? 
O2 Y1 Fe1 O1 126.22(15) 5_767 . . 5_767 ? 
O2 Y1 Fe1 O1 62.02(14) 3_747 . . 5_767 ? 
O2 Y1 Fe1 O1 -3.05(14) 4_456 . . 5_767 ? 
O2 Y1 Fe1 O1 -118.34(15) 6_557 . . 5_767 ? 
Mn1 Y1 Fe1 O1 0(70) . . . 5_767 ? 
Fe1 Y1 Fe1 O1 23.49(13) 3_747 . . 5_767 ? 
Mn1 Y1 Fe1 O1 23.49(13) 3_747 . . 5_767 ? 
O1 Y1 Fe1 O1 104.41(11) 2_664 . . . ? 
O2 Y1 Fe1 O1 -80.70(19) 8_756 . . . ? 
O2 Y1 Fe1 O1 0.49(14) 2_665 . . . ? 
O1 Y1 Fe1 O1 180.0 5_767 . . . ? 
O2 Y1 Fe1 O1 -53.78(15) 5_767 . . . ? 
O2 Y1 Fe1 O1 -117.98(13) 3_747 . . . ? 
O2 Y1 Fe1 O1 176.95(14) 4_456 . . . ? 
O2 Y1 Fe1 O1 61.66(15) 6_557 . . . ? 
Mn1 Y1 Fe1 O1 0(18) . . . . ? 
Fe1 Y1 Fe1 O1 -156.51(13) 3_747 . . . ? 
Mn1 Y1 Fe1 O1 -156.51(13) 3_747 . . . ? 
O1 Y1 Fe1 O2 42.75(9) 2_664 . . 6_557 ? 
O2 Y1 Fe1 O2 -142.36(17) 8_756 . . 6_557 ? 
O2 Y1 Fe1 O2 -61.17(12) 2_665 . . 6_557 ? 
O1 Y1 Fe1 O2 118.34(15) 5_767 . . 6_557 ? 
O2 Y1 Fe1 O2 -115.44(6) 5_767 . . 6_557 ? 
O2 Y1 Fe1 O2 -179.64(12) 3_747 . . 6_557 ? 
O2 Y1 Fe1 O2 115.29(12) 4_456 . . 6_557 ? 
Mn1 Y1 Fe1 O2 0(12) . . . 6_557 ? 
Fe1 Y1 Fe1 O2 141.83(8) 3_747 . . 6_557 ? 
Mn1 Y1 Fe1 O2 141.83(8) 3_747 . . 6_557 ? 
O1 Y1 Fe1 O2 -137.25(9) 2_664 . . 2_765 ? 
O2 Y1 Fe1 O2 37.64(17) 8_756 . . 2_765 ? 
O2 Y1 Fe1 O2 118.83(12) 2_665 . . 2_765 ? 
O1 Y1 Fe1 O2 -61.66(15) 5_767 . . 2_765 ? 
O2 Y1 Fe1 O2 64.56(6) 5_767 . . 2_765 ? 
O2 Y1 Fe1 O2 0.36(12) 3_747 . . 2_765 ? 
O2 Y1 Fe1 O2 -64.71(12) 4_456 . . 2_765 ? 
O2 Y1 Fe1 O2 180.0 6_557 . . 2_765 ? 
Mn1 Y1 Fe1 O2 0(75) . . . 2_765 ? 
Fe1 Y1 Fe1 O2 -38.17(8) 3_747 . . 2_765 ? 
Mn1 Y1 Fe1 O2 -38.17(8) 3_747 . . 2_765 ? 
O1 Y1 Fe1 Y1 78(17) 2_664 . . 5_767 ? 
O2 Y1 Fe1 Y1 -107(17) 8_756 . . 5_767 ? 
O2 Y1 Fe1 Y1 -26(17) 2_665 . . 5_767 ? 
O1 Y1 Fe1 Y1 154(17) 5_767 . . 5_767 ? 
O2 Y1 Fe1 Y1 -80(17) 5_767 . . 5_767 ? 
O2 Y1 Fe1 Y1 -144(17) 3_747 . . 5_767 ? 
O2 Y1 Fe1 Y1 151(17) 4_456 . . 5_767 ? 
O2 Y1 Fe1 Y1 35(17) 6_557 . . 5_767 ? 
Mn1 Y1 Fe1 Y1 0(67) . . . 5_767 ? 
Fe1 Y1 Fe1 Y1 177(17) 3_747 . . 5_767 ? 
Mn1 Y1 Fe1 Y1 177(17) 3_747 . . 5_767 ? 
O1 Y1 Fe1 Y1 24.34(6) 2_664 . . 2_664 ? 
O2 Y1 Fe1 Y1 -160.78(16) 8_756 . . 2_664 ? 
O2 Y1 Fe1 Y1 -79.59(6) 2_665 . . 2_664 ? 
O1 Y1 Fe1 Y1 99.93(13) 5_767 . . 2_664 ? 
O2 Y1 Fe1 Y1 -133.85(9) 5_767 . . 2_664 ? 
O2 Y1 Fe1 Y1 161.95(5) 3_747 . . 2_664 ? 
O2 Y1 Fe1 Y1 96.87(5) 4_456 . . 2_664 ? 
O2 Y1 Fe1 Y1 -18.41(8) 6_557 . . 2_664 ? 
Mn1 Y1 Fe1 Y1 0(21) . . . 2_664 ? 
Fe1 Y1 Fe1 Y1 123.413(5) 3_747 . . 2_664 ? 
Mn1 Y1 Fe1 Y1 123.413(5) 3_747 . . 2_664 ? 
O1 Y1 Fe1 Y1 -155.66(6) 2_664 . . 6_658 ? 
O2 Y1 Fe1 Y1 19.22(16) 8_756 . . 6_658 ? 
O2 Y1 Fe1 Y1 100.41(6) 2_665 . . 6_658 ? 
O1 Y1 Fe1 Y1 -80.07(13) 5_767 . . 6_658 ? 
O2 Y1 Fe1 Y1 46.15(9) 5_767 . . 6_658 ? 
O2 Y1 Fe1 Y1 -18.05(5) 3_747 . . 6_658 ? 
O2 Y1 Fe1 Y1 -83.13(5) 4_456 . . 6_658 ? 
O2 Y1 Fe1 Y1 161.59(8) 6_557 . . 6_658 ? 
Mn1 Y1 Fe1 Y1 0(66) . . . 6_658 ? 
Fe1 Y1 Fe1 Y1 -56.587(5) 3_747 . . 6_658 ? 
Mn1 Y1 Fe1 Y1 -56.587(5) 3_747 . . 6_658 ? 
O1 Y1 Fe1 Y1 -42.84(6) 2_664 . . 6_657 ? 
O2 Y1 Fe1 Y1 132.05(15) 8_756 . . 6_657 ? 
O2 Y1 Fe1 Y1 -146.76(6) 2_665 . . 6_657 ? 
O1 Y1 Fe1 Y1 32.75(13) 5_767 . . 6_657 ? 
O2 Y1 Fe1 Y1 158.97(9) 5_767 . . 6_657 ? 
O2 Y1 Fe1 Y1 94.78(5) 3_747 . . 6_657 ? 
O2 Y1 Fe1 Y1 29.70(5) 4_456 . . 6_657 ? 
O2 Y1 Fe1 Y1 -85.59(8) 6_557 . . 6_657 ? 
Mn1 Y1 Fe1 Y1 0(54) . . . 6_657 ? 
Fe1 Y1 Fe1 Y1 56.238(6) 3_747 . . 6_657 ? 
Mn1 Y1 Fe1 Y1 56.238(6) 3_747 . . 6_657 ? 
O1 Y1 Fe1 Y1 137.16(6) 2_664 . . 2_665 ? 
O2 Y1 Fe1 Y1 -47.95(15) 8_756 . . 2_665 ? 
O2 Y1 Fe1 Y1 33.24(6) 2_665 . . 2_665 ? 
O1 Y1 Fe1 Y1 -147.25(13) 5_767 . . 2_665 ? 
O2 Y1 Fe1 Y1 -21.03(9) 5_767 . . 2_665 ? 
O2 Y1 Fe1 Y1 -85.22(5) 3_747 . . 2_665 ? 
O2 Y1 Fe1 Y1 -150.30(5) 4_456 . . 2_665 ? 
O2 Y1 Fe1 Y1 94.41(8) 6_557 . . 2_665 ? 
Mn1 Y1 Fe1 Y1 0(34) . . . 2_665 ? 
Fe1 Y1 Fe1 Y1 -123.762(6) 3_747 . . 2_665 ? 
Mn1 Y1 Fe1 Y1 -123.762(6) 3_747 . . 2_665 ? 
 
_diffrn_measured_fraction_theta_max    1.000 
_diffrn_reflns_theta_full              24.99 
_diffrn_measured_fraction_theta_full   1.000 
_refine_diff_density_max    0.315 
_refine_diff_density_min   -0.586 
_refine_diff_density_rms    0.123 
